FiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens


 Damon Willis
 1 years ago
 Views:
Transcription
1 Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: FiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens ABSTRACT: Experimental results showed that ASTM D 638 Type IV flat tension specimens, made of a Nylon11 matrix containing a large volume concentration of NdFeB particulates, failed at a location where the straight gage section of the specimen ends and the curved transition region begins. The stress distribution in this specimen was analyzed using the finiteelement method, and it was found that there is a stress concentration at this location. The stress distributions in tension specimens with both single and doublearc transition regions were analyzed and stress concentration factors were calculated. A linear relationship between the magnitude of the stress concentration factor and the ratio of the width in the gage section and the arc radius of the transition region is identified. This study shows that it is possible to reduce the magnitude of the stress concentration factor for the ASTM D 638 Type IV flat tension specimen by redesigning the specimen geometry without changing its overall size. KEYWORDS: stress concentration factor, finiteelement analysis, tensile strength Recent advancements in injection molding have made it a popular manufacturing method for costeffective, highvolume production of plastic and particlereinforced plastic composites. ASTM Standard D 638 [1], a standard test method for tensile strength of plastics, has been used widely in the industry to evaluate the tensile strength of plasticbased materials. In the absence of test methods for the tensile evaluation of particulatereinforced plastics, the ASTM D 638 test method also has been used to evaluate these reinforced plastic composites. Figure 1a shows a fractured ASTM D 638 Type IV specimen made of Nylon11 bonded NdFeB particles. This material, which contains 59.7 vol% of brittle NdFeB particles, is formulated for permanent magnet applications. The high percentage of NdFeB particles is necessary to achieve the desired magnetic properties for electrical motor and actuator applications. However, the high percentage of NdFeB particles also results in a material with reduced ductility [2 4]. The tensile evaluation of plasticbonded NdFeB magnets has shown that fracture almost always initiates at a location where the straight gage section of the specimen ends and the curved transition region begins. This location is marked as Point B in Fig. 1a. The failure at Point B, which is outside the uniformly loaded straight gage section, is due to a stress concentration and can lead to an underestimate of the tensile strength. Such stress concentration is not a problem for ductile materials because the large plastic deformation will redistribute the stress. For example, Fig. 1b shows a deformed ASTM D 638 Type IV tension specimen made of pure Nylon11. This specimen continued to deform extensively without fracturing at the location of initial stress concentration. Manuscript received 5/2/2002; accepted for publication 11/13/2002; published 11/18/ Department of Mechanical and Aerospace Engineering, North Carolina State University, Raleigh, NC Department of Mechanical Engineering, University of Michigan, Ann Arbor, MI High Temperature Materials Laboratory, Oak Ridge National Laboratory, Oak Ridge, TN Department of Materials Science and Engineering, North Carolina State University, Raleigh, NC As engineered and particlereinforced plastics become stronger and in some cases more brittle, the stress concentration in current tension specimen geometries has become an issue of concern. One of the objectives in this research is to analyze the stress concentration factor [5] on specimens specified in ASTM D 638 using the finiteelement method. Five types of specimens, designated as Type I, II, III, IV, and V, are defined in ASTM D 638. The shapes of Type III and V specimens are similar, which results in the same stress concentration factor at the location where the gage section ends and the transition region begins. Therefore, only Type I, II, III, and IV specimens were studied. In addition to these four standard tension specimens, the stress concentration factor for other specimen geometries with single or doublearc fillets was also analyzed using the finiteelement method to investigate possible ways to reduce the stress concentration without changing the overall size of specimens. The photoelastic method has been used in the past to study the stress concentration factors for shoulder fillets in flat plates [5 7]. Most of the cases studied have fillet radii much smaller than the width of the specimen. The shapes of tension specimens investigated in this research have the opposite trend: the fillet radii are much larger than the width of the specimen in order to reduce the stress concentration factor. For specimens with very small stress concentration factors, the finiteelement method with a reasonably fine mesh was applied to analyze the stress distributions and estimate the stress concentration factors. The finiteelement method has been applied previously to the design of flat tension specimens of advanced composites [8], ceramic matrix composites [9], and monolithic ceramics for creep testing [10]. Oplinger et al. [11] has studied the use of streamlined specimens to reduce the tensile and shear stress concentration in composite specimens. In this paper, first the finiteelement modeling of tension specimens is introduced. The stress concentration factor is defined. The distribution of von Mises stresses for four types of specimens specified in ASTM Standard D 638 is presented. The stress concentration factors of other specimen shapes with single and doublearc fillets are analyzed. Finally, a correlation between the magnitude of the stress concentration factor and the ratio of arc radius and width of the gage section is established. Copyright 2003 by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA
2 2 JOURNAL OF TESTING AND EVALUATION FiniteElement Modeling The twodimensional plane stress sixnode and twelve degreeoffreedom triangular linear elastic element was selected to model the flatplate tension specimens. The commercially available AN SYS finiteelement analysis software and its mesh generator were used. Figure 2 shows the finiteelement meshes used to model the four types of ASTM D 638 tension specimens. Due to the symmetry of the specimen geometry, only one quarter of the specimen is modeled. Point O is the center of the specimen. Lines OA and OE are the symmetry planes of the specimen. Point O is fixed in both the X and Ydirections. Nodes on Line OA have zero displacement in the Xdirection and are free to move in the Ydirection. Nodes on Line OE have zero displacement in the Ydirection and are free to move in the Xdirection. Nodes on Line ED are prescribed a uniform 0.1mm displacement in the Xdirection and zero displacement in the Ydirection. This is intended to simulate the holding of both ends in the wide section of the tension specimen using perfectly rigid grips. The extension of the specimen under this condition is 0.2 mm. In actual tensile tests, the specimen is clamped and pulled using a set of mechanical or hydraulic grips. The actual loading condition near the gripped area is therefore the combination of the normal compressive stress and inplane tensile and shear stresses. Dimensions of finiteelement meshes and the number of elements and nodes are summarized in the table in Fig. 2 for each type of ASTM D 638 specimen. OA is one half of the width of the gage FIG. 1 Pictures of ASTM D Type IV tension specimens: (a) Nylon11 bonded NdFeB (59.7 vol%) material tested with at 100 C, and (b) pure Nylon11 tested at 100 C. FIG. 3 Geometric model of the single and double radius transitional area. FIG. 2 Finiteelement mesh for four types of specimen in ASTM D
3 GARRELL ET AL. ON ASTM 638 TEST SPECIMENS 3 FIG. 4 Distribution of von Mises stress in ASTM D 638 tensile test specimens. (Value by the node represents the ratio of nodal von Mises stress relative to the maximum von Mises stress at node MX in Pa.) section, DE is one half of the width of the wide section, OE is one half of the length of the specimen, and AB is one half of the length of the gage section. Between Points B and C, the specimen changes from the narrow to the wide section. As shown in Figs. 2a, 2b, and 2c, Type I, II, and III specimens consist of a circular arc of radius r 1 between Points B and C. These are known as singlearc specimens. As shown in Fig. 2d, two radii, r 1 and r 2, are used to blend two arcs in the transitional region between Points B and C for the Type IV specimen. This is designated as the doublearc specimen. The geometrical relationships of the single and doublearc shape between Points B and C are shown in Fig. 3; w 1 and w 2 are widths of the narrow and wide section, respectively. As shown in Fig. 3a, the singleradius specimen has a continuous slope at Point B and a discontinuous slope at Point C. The doublearc specimen, as shown in Fig. 3b, has a continuous slope at all three transitional points: B, F, and C. Arcs BF and FC have the same angle, indicated by. The center of Arc BF, denoted as C 1 in Fig. 3a, has the same Xcoordinate as Point B. Similarly, the center of Arc CF, denoted as C 2, has the same Xcoordinate as Point C. These geometrical constraints together ensure a continuous slope at Points B, F, and C for the doublearc specimen. A hydrostatic stressdependent yield criterion is usually used to analyze stress concentrations in plastics [12,13]. The yield criterion for magnetic particle reinforced plastics has not yet been studied. The maximum von Mises stress was used to calculate the stress concentration factor and to identify the location that possibly initializes the fracture. In addition to the von Mises stress, the maximum principal stress, which is more suitable for the analysis of brittle materials, was also applied to calculate the stress concentration factor. The finiteelement analysis provided results of stress components and the von Mises and principal stress for each node. The nodal stress was used to calculate the stress concentration factor, K f. max K f (1) nominal where max is either the maximum nodal von Mises stress or maximum first principal stress, and nominal is either the average von Mises stress or the average first principal stress on nodes in the gage section. Finiteelement analysis results show that the variation of von Mises stress among nodes in the gage section is very small, less than 1.5%. An elastic modulus of 130 MPa and Poisson s ratio of 0.3 were used in the finiteelement analysis.
4 4 JOURNAL OF TESTING AND EVALUATION FiniteElement Analysis of Four Types of Tension Specimens Figure 4 shows the distribution of von Mises stress for ASTM D 638 Type I, II, III, and IV standard tension specimens. For each specimen, an overview and another enlarged view of the von Mises TABLE 1 The stress concentration for different single and doubleradius tension specimen geometry. Designation r 1 (mm) r 2 (mm) w 1 /r 1 K f ASTM Type I D 638 Type II Type III Type IV Single SI radius SII tension SIII specimen SIV SV SVI SVII Double DI radius DII* tension DIII specimen DIV DV DVI DVII * The same geometry as Type IV. stress distribution is presented. The enlarged view is centered about Point B to identify the increase in von Mises stress. In Fig. 4, MX and MN mark the nodes with maximum and minimum von Mises stress, respectively. As shown in the overview of the specimen, Node MN is close to Point C. In the enlarged view, the location of Node MX relative to Node B can be seen. Node MX is next to Node B, as in Type I and II, or a node away from Node B, as in Type III and IV. It is noted that the mesh shown in the enlarged view represents the exaggeratedly deformed finiteelement mesh from the ANSYS output. Node B, originally located at the intersection of a straight line and an arc, can be seen on a slightly curved region after deformation. The ratio of nodal von Mises stress relative to the maximum von Mises stress at Node MX is also presented in the enlarged view on nodes around Points B and MX in Fig. 4. For Type I, II, and III specimens, the overview of von Mises stress distribution does not show the stress concentration. Upon closely examining the distribution of von Mises stress around Point MX in the enlarged view, all four types of ASTM D 638 tension specimens demonstrate different levels of stress concentration at Node MX. The von Mises stress at Node MX ( max ) and at nodes in the gage section ( nominal ) were extracted from the finiteelement output and substituted into Eq 1 to calculate the stress concentration factor, K f. Results of K f are listed in Table 1. Type IV and II specimens have the highest and lowest K f, and 1.014, respectively. It was found that K f has an almost linear relationship versus the parameter w 1 /r 1, as shown in Fig. 5, for the four types of ASTM D 638 specimen. FIG. 5 The stress concentration factor versus ratio of gage section width and radius for five types of ASTM D 638 specimens and the single and doubleradius specimens.
5 GARRELL ET AL. ON ASTM 638 TEST SPECIMENS 5 Tension specimens with low w 1 /r 1 ratio usually have large arc radius and are longer than specimens with high w 1 /r 1. For example, as shown in Fig. 2 and Table 1, Type II and IV specimens have the same width in the gage section and different radius r 1. The Type II specimen has a larger arc radius, which makes the specimen longer and has lower w 1 /r 1 and K f. Longer and bigger tension specimens are unattractive because they require more material and a bigger die for injection molding and cost more to produce. Instead of using the von Mises stress, the maximum principal stress and nominal principal stress were extracted from the finiteelement output and substituted into Eq 1 to calculate K f. For all four types of specimens, the difference in K f based on von Mises and maximum principal stresses is very small, less than FiniteElement Analysis of Single and DoubleArc Tension Specimens In this section, the investigation of stress distribution in alternative tension specimen geometries that maintain the same overall size as the Type IV specimen is discussed. The objective is to identify the geometric parameters that would reduce the magnitude of K f. The width (w 1 ) and length of the gage section are 6 and 13 mm, respectively. The width of the wide section, w 2, is 19 mm. Two groups of sample geometry were studied. One group consists of singlearc specimens, similar to those in Type I, II, and III. Another group has the doublearc geometry, similar to the Type IV specimen. SingleArc Specimens As shown in Table 1, seven single radius curves are used to blend between Points B and C. The minimum radius of Arc BC is 6.5 mm ( (w 2 w 1 )/2). The specimens with radii of 6.5, 9, 13, 19, 28, 39, or 52 mm at Arc BC were designated as SI to SVII, respectively. The shape and finiteelement mesh of three selected specimens, SI, SIV, and SVII, are shown in Fig. 6. For specimens with arc radius equal to or less than 39 mm, the overall length of the original Type IV specimen can be maintained. The K f of the 39mm radius singlearc specimen (SVI), as shown in Table 1, is This is significantly lower than K f of of the Type IV specimen. Plots of K f versus w 1 /r 1 for these seven specimens are shown in Fig. 5. The larger radius of arc BC lowers both w 1 /r 1 and K f. Figure 5 also shows that the relationship between K f and w 1 /r 1 is almost linear and matches the trend of Type I to IV specimens. DoubleArc Specimens Seven doublearc specimens, denoted as DI to DVII, were studied as well. As shown in Fig. 3, the values of r 1 and r 2 in the doublearc geometry can be reversed and still maintain the continuity of both position and slope at Points B, F, and C. This special geometrical characteristic of the doublearc shape was used to define conjugate pairs of specimens. As shown in Table 1, DI (r 1 9 mm, r 2 30 mm) and DVII (r 1 30 mm, r 2 9 mm) form a conjugate pair of doublearc specimens. DII (r 1 14 mm, r 2 25 mm) and DVI (r 1 25 mm, r 2 14 mm) as well as DIII (r 1 17 mm, r 2 22 mm) and DV (r 1 22 mm, r 2 17 mm) are another two sets of conjugate doublearc specimens. It is noted that the DII specimen has the same geometry as the ASTM D 638 Type IV specimen. The intent is to investigate the change in K ƒ of a conjugate doublearc specimen. The DIII specimen has the same r 1 and r 2, both equal to 19.5 mm. The shape and finiteelement mesh of three selected specimens, DI, DIV, and DVII, are shown in Fig. 6. Finiteelement analysis results of K f versus w 1 /r 1 for seven doublearc specimens are listed in Table 1 and plotted in Fig. 5. It is important to note that the value of r 2 does not affect K f. By just switching the two arcs of the original Type IV specimen, the K f was reduced from to By further increasing r 1 to 30 mm without changing the overall size of the Type IV specimen, K f was reduced to Modeling of the Stress Concentration Factor As shown in Fig. 5, a straight line can be used to determine K f for various w 1 /r 1. Linear regression analysis was performed on all 17 data points, including the four types of specimen specified by ASTM D 638 and the seven singlearc and six doublearc specimens. The following model is obtained: K f (w 1 /r 1 ) (2) Equation 2 can be used to predict the K f based on w 1 /r 1 and may be useful for new tension specimen design. FIG. 6 Finiteelement meshes for selected single and doublearc specimens (3 mm halfwidth in the gage section for all specimens).
6 6 JOURNAL OF TESTING AND EVALUATION The linear trend indicates the possibility that an analytical solution for the stress distribution in this geometrical configuration may exist. This requires further investigation. Concluding Remarks The stress distribution of four types of tension specimens recommended in ASTM D 638 was investigated through the use of the finiteelement technique. It was found that the location of maximum von Mises stress for Type IV geometry coincided with the location of experimentally observed failures in brittle specimens made of Nylon11 bonded NdFeB particles. This study identified a solution to reduce the magnitude of stress concentration by increasing the radius of the arc in the transitional area. A linear correlation of stress concentration factor K f versus w 1 /r 1 was identified and a linear model was established to predict the K f based on w 1 /r 1. Results obtained in this research can help establish standards and aid in the design of specimen geometry for tension testing of brittle particlereinforced composites. Acknowledgments A portion of this research was sponsored by the User program of the High Temperature Material Laboratory of Oak Ridge National Laboratory and by National Science Foundation Grant (Dr. K. P. Rajurkar, Program Director). References [1] ASTM D : Standard Test Method for Tensile Strength of Plastics, Annual Book of ASTM Standards, ASTM International, West Conshohocken, PA, [2] Garrell, M. G., Ma, B. M., LaraCurzio, E., Shih, A. J., and Scattergood, R. O., Mechanical Properties of Nylon Bonded NdFeB Permanent Magnets, Journal of Magnetism and Magnetic Materials, accepted for publication. [3] Garrell, M. G., Ma, B. M., LaraCurzio, E., Shih, A. J., and Scattergood, R. O., Mechanical Properties of PolyphenyleneSulfide (PPS) Bonded NdFeB Permanent Magnets, Materials Science and Engineering: A, submitted. [4] Garrell, M. G., Mechanical Properties of Injection Molded Permanent Magnets, M.S. thesis, North Carolina State University, Raleigh, NC, April [5] Pilkey, W. D., Peterson s Stress Concentration Factors, 2nd ed., John Wiley & Sons, New York, [6] Wilson, L. H. and White, D. J. StressConcentration Factors for Shoulder Fillets and Grooves in Plates, Journal of Strain Analysis, Vol. 8, 1973, pp [7] Frocht, M. M. Factor of Stress Concentration Photoelastically Determined, Transactions of ASME, 1935, Vol. 57, pp. A67 A68. [8] Worthem, D. W., Flat Tension Specimen Design for Advanced Composites, NASA Technical Report CR , NASA Lewis Research Center, Cleveland, OH, [9] Shi, J., Brady, L., and Ireson, A., Design of Room Temperature Tension Specimen Made of Ceramic Matrix Composites, Key Engineering Materials, Vol , Trans Tech Publications, 1999, pp [10] Wang, Z, Chiang, C. K., and Chuang, T.J., Optimum Design of a Ceramic Tensile Creep Specimen Using a Finite Element Method, Journal of Research of the National Institute of Standards and Technology, Vol. 102, 1997, pp [11] Oplinger, D. W., Parker, B. S., Gandhi, K. R., Lamothe, R., and Foley, G., On the Streamline Specimen for Tension Testing of Composite Materials, Recent Advances in Composites in the United States and Japan, ASTM STP 864, J. R. Vinson and M. Taya, Eds., ASTM International, West Conshohocken, PA, 1985, pp [12] McCrum, N. G., Buckley, C. P., and Bucknall, C. B., Principles of Polymer Engineering, 2nd ed., Oxford University Press, Oxford, [13] Courtney, T. H., Mechanical Behavior of Materials, 2nd ed., McGrawHill, New York, 2000.
Structural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature
Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment TiniusOlsen LoTorq Torsion Machine (figure
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More informationIMECE CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT
Proceedings of IMECE04 2004 ASME International Mechanical Engineering Congress November 1320, 2004, Anaheim, California USA IMECE200460700 CRACK TUNNELING: EFFECT OF STRESS CONSTRAINT Jianzheng Zuo Department
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationStandard Test Methods for GlassBonded Mica Used as Electrical Insulation 1
Designation: D 1039 94 (Reapproved 1999) e1 An American National Standard Standard Test Methods for GlassBonded Mica Used as Electrical Insulation 1 This standard is issued under the fixed designation
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationEffect Of The InSitu Stress Field On Casing Failure *
Effect Of The InSitu Stress Field On Casing Failure * Tang Bo Southwest Petroleum Institute, People's Republic of China Lian Zhanghua Southwest Petroleum Institute, People's Republic of China Abstract
More informationLife Prediction Under Multiaxial Fatigue
Lie Prediction Under Multiaxial Fatigue D. Ramesh and M.M. Mayuram Department o Mechanical Engineering Indian Institute o Technology, Madras Chennai600 036 (India) email: mayuram@iitm.ac.in ABSTRACT
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationFinite Element Analysis of Bicycle Crank
IJSTE  International Journal of Science Technology & Engineering Volume 3 Issue 10 April 2017 ISSN (online): 2349784X Finite Element Analysis of Bicycle Crank Mohammed Asif Kattimani Assistant Professor
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationFinite Element Analysis of Compression of Thin, High Modulus, Cylindrical Shells with LowModulus Core
Finite Element Analysis of Compression of Thin, High Modulus, Cylindrical Shells with LowModulus Core Robert S. Joseph Design Engineering Analysis Corporation, McMurray, PA ABSTRACT Long, cylindrical
More informationStudy of Circular and Elliptical Holes as a Stress Relieving Feature in Spur Gear
Study of Circular and Elliptical Holes as a Stress Relieving Feature in Spur Gear Prof. S.B.Naik 1, Mr. Sujit R. Gavhane 2 Asst. Prof. Department of Mechanical Engineering, Walchand Institute of Technology,
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationLINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL
LINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL SREELATHA P.R * M.Tech. Student, Computer Aided Structural Engineering, M A College of Engineering, Kothamangalam 686 666,
More informationElastic Properties of Solid Materials. Notes based on those by James Irvine at
Elastic Properties of Solid Materials Notes based on those by James Irvine at www.antonineeducation.co.uk Key Words Density, Elastic, Plastic, Stress, Strain, Young modulus We study how materials behave
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationTolerance Ring Improvement for Reducing Metal Scratch
International Journal of Scientific and Research Publications, Volume 2, Issue 11, November 2012 1 Tolerance Ring Improvement for Reducing Metal Scratch Pattaraweerin Woraratsoontorn*, Pitikhate Sooraksa**
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationFinal Design Project: Biodiesel Settling Tank Analysis
MESSIAH COLLEGE ENGR 495 Finite Element Methods Tuesday, December 16, 2003 : Biodiesel Settling Tank Analysis Brandon Apple Jon Bitterman Becky Gast Kyle McNamara ENGR 495 Finite Element Methods 1 Abstract
More informationThis guide is made for nonexperienced FEA users. It provides basic knowledge needed to start your fatigue calculations quickly.
Quick Fatigue Analysis Guide This guide is made for nonexperienced FEA users. It provides basic knowledge needed to start your fatigue calculations quickly. Experienced FEA analysts can also use this
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationFatigue Algorithm Input
Methods Fatigue Algorithm Input By default, fesafe analyses stress datasets that contain elastic stresses The calculation of elasticplastic stressstrains, where necessary, is performed in fesafe using
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationFigure 1: Throwing arm dimensions
I. Overview The objective of this report is to review the design of the trebuchet model from an engineering standpoint. This study analyzes the dimensions and material selection using the COMSOL multiphisics
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationDESIGN OF GRIPPER IN UNIVERSAL TESTING MACHINE
DESIGN OF GRIPPER IN UNIVERSAL TESTING MACHINE BAIJU R DABHI 1, PROF.(DR.) V. D. CHAUHAN 2, PROF.P.G.CHOKSI 3 1 M.E. (Machine Design), Department of Mechanical Engineering, B.V.M Engineering College, V.V.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationFigure 1 Lifting Lug Geometry with Weld
Should you Perform Nonlinear Stress Analysis? Many of our clients inquire whether nonlinearity should be considered in their analyses. The answer to that question is not simple. Sometimes, as in certain
More informationASSESSMENT OF DYNAMICALLY LOADED CRACKS IN FILLETS
ASSESSMENT OF DNAMICALL LOADED CRACKS IN FILLETS Uwe Zencker, Linan Qiao, Bernhard Droste Federal Institute for Materials Research and Testing (BAM) 12200 Berlin, Germany email: zencker@web.de Abstract
More informationContact Modeling of Rough Surfaces. Robert L. Jackson Mechanical Engineering Department Auburn University
Contact Modeling of Rough Surfaces Robert L. Jackson Mechanical Engineering Department Auburn University Background The modeling of surface asperities on the microscale is of great interest to those interested
More informationConcept Question Comment on the general features of the stressstrain response under this loading condition for both types of materials
Module 5 Material failure Learning Objectives review the basic characteristics of the uniaxial stressstrain curves of ductile and brittle materials understand the need to develop failure criteria for
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationImproved stress prediction in adhesive bonded optical components
Improved stress prediction in adhesive bonded optical components J. de Vreugd 1a, M.J.A. te Voert a, J.R. Nijenhuis a, J.A.C.M. Pijnenburg a, E. Tabak a a TNO optomechatronics, Stieltjesweg 1, 2628 CK,
More informationThe design of a formula student front impact attenuator
The design of a formula student front impact attenuator J.M.J. Schormans MT 10.06 Supervisors: dr. ir. Varvara Kouznetsova Eindhoven University of Technology Department of Mechanical Engineering Computational
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationINVESTIGATION OF STRESSES IN FLAT BELT PULLEY BY FEM AND PHOTOELASTICITY
INVESTIGATION OF STRESSES IN FLAT BELT PULLEY BY FEM AND PHOTOELASTICITY * N. W. Pathan, **Dr. D.V. Bhope, *** Prof. S.D Khamankar Abstract * Department of Mech. Engg., Rajiv Gandhi College of Engineering
More informationStrength of Adhesive Joints: A Parametric Study
Project PAJex1  Report 3 Strength of Adhesive Joints: A Parametric Study W R Broughton, L E Crocker and J M Urquhart July 2001 NPL Materials Centre National Physical Laboratory NPL Report MATC(A)27 July
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationAn exact reanalysis algorithm using incremental Cholesky factorization and its application to crack growth modeling
INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING Int. J. Numer. Meth. Engng 01; 91:158 14 Published online 5 June 01 in Wiley Online Library (wileyonlinelibrary.com). DOI: 10.100/nme.4 SHORT
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationRESEARCH PROJECT NO. 26
RESEARCH PROJECT NO. 26 DETERMINATION OF POISSON'S RATIO IN AD1 TESTING BY UNIVERSITY OF MICHIGAN REPORT PREPARED BY BELA V. KOVACS and JOHN R. KEOUGH \ MEMBER / / DUCTILE IRON \ SOCIETY Issued by the
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationSolid Mechanics Homework Answers
Name: Date: Solid Mechanics Homework nswers Please show all of your work, including which equations you are using, and circle your final answer. Be sure to include the units in your answers. 1. The yield
More information3 A y 0.090
ROBLM.1 5.0 in. 5 8 in. diameter A standard tension test is used to determine the properties of an experimental plastic. The test specimen is a 5 in.diameter rod and it is subjected to an 800lb tensile
More informationA *69>H>N6 #DJGC6A DG C<>C::G>C<,8>:C8:H /DA 'D 2:6G  (  ) +"' ( + "( (' (& +" % '('%"' +"2 ( !"', % )% .C>K:GH>IN D; AF69>HH>6,+
The primary objective is to determine whether the structural efficiency of plates can be improved with variable thickness The large displacement analysis of steel plate with variable thickness at direction
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationChapter 5. Vibration Analysis. Workbench  Mechanical Introduction ANSYS, Inc. Proprietary 2009 ANSYS, Inc. All rights reserved.
Workbench  Mechanical Introduction 12.0 Chapter 5 Vibration Analysis 51 Chapter Overview In this chapter, performing free vibration analyses in Simulation will be covered. In Simulation, performing a
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationStrain Distribution and Load Transfer in the PolymerWood Particle Bond in Wood Plastic Composites
Strain Distribution and Load Transfer in the PolymerWood Particle Bond in Wood Plastic Composites Matthew J. Schwarzkopf Lech Muszyński John Nairn Department of Wood Science and Engineering, Oregon State
More informationArberi Ferraj. Wentworth Institute of Technology. Design of Machine Elements MECH 420
P a g e 1 Arberi Ferraj Wentworth Institute of Technology Design of Machine Elements MECH 420 P a g e 2 1. Executive Summary A scissor car jack was designed and must be reverseengineered in order to discover
More informationCSCE 155N Fall Homework Assignment 2: StressStrain Curve. Assigned: September 11, 2012 Due: October 02, 2012
CSCE 155N Fall 2012 Homework Assignment 2: StressStrain Curve Assigned: September 11, 2012 Due: October 02, 2012 Note: This assignment is to be completed individually  collaboration is strictly prohibited.
More informationAvailable online at Fatigue Fatigue life prediction for large threaded components. Ali Cetin*, Gunnar Härkegård
Available online at www.sciencedirect.com Procedia Procedia Engineering Engineering 2 (2010) 00 (2009) 1225 1233 000 000 Procedia Engineering www.elsevier.com/locate/procedia Fatigue 2010 Fatigue life
More information22 Which of the following correctly defines the terms stress, strain and Young modulus? stress strain Young modulus
PhysicsndMathsTutor.com Which of the following correctly defines the terms stress, strain and Young modulus? 97/1/M/J/ stress strain Young modulus () x (area) (extension) x (original length) (stress) /
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationTINIUS OLSEN Testing Machine Co., Inc.
Interpretation of StressStrain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stressstrain curves for the benefit of those
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationLowCycle Fatigue Crack Growth in Ti6242 at Elevated Temperature Rebecka Brommesson 1,a, Magnus Hörnqvist,2,b, and Magnus Ekh 3,c
LowCycle Fatigue Crack Growth in Ti6242 at Elevated Temperature Rebecka Brommesson 1,a, Magnus Hörnqvist,2,b, and Magnus Ekh 3,c 1,3 Department of Applied Mechanics, Chalmers University of Technology,
More informationSimulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias
As originally published in the IPC APEX EXPO Conference Proceedings. Simulation of the Influence of Manufacturing Quality on Thermomechanical Stress of Microvias Yan Ning, Michael H. Azarian, and Michael
More informationBasics of Finite Element Analysis. Strength of Materials, Solid Mechanics
Basics of Finite Element Analysis Strength of Materials, Solid Mechanics 1 Outline of Presentation Basic concepts in mathematics Analogies and applications Approximations to Actual Applications Improvisation
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationNumerical simulation the bottom structures. grounding test by LSDYNA
5 th European LSDYNA Users Conference Methods and Techniques (3) Numerical simulation the bottom structures grounding test by LSDYNA Ainian Zhang Graduate School of Frontier Sciences, The University
More information